Birefringent all-solid hybrid microstructured fiber

We report the characterization of a birefringent all-solid hybrid microstructured fiber, in which the core-modes are guided by both the photonic bandgap (PBG) effect and total internal reflection (TIR). Due to the twofold symmetry, modal birefringence of 1 .5× 10−4 and group birefringence of 2.1× 10−4 were measured at 1.31 μm, which is in the middle of the second bandgap. The band structure was calcula ted to be different from conventional 2-D PBG fibers due to the 1-D arra ngement of high-index regions. The bend loss has a strong directiona l dependence due to the coexistence of the two guiding mechanisms. The fibe r has two important properties pertinent to PBG fibers; spectral fi ltering, and chromatic dispersion specific to PBG fibers. The number of hig h-index regions, which trap pump power (by index guiding) when the fib er is used in cladding-pumped fiber lasers, is greatly reduced so t hat this fiber should enable efficient cladding pumping. This structure is suitable for linearly-polarized, cladding-pumped fiber lasers utilizi ng the properties of PBG fibers. © 2008 Optical Society of America OCIS codes:(060.2310) fiber optics; (060.2400) fiber properties. References and links 1. F. Brechet, P. Roy, J. Marcou, and D. Pagnoux, “Single-mode propagation into depressed-core-index photonicbandgap fibre designed for zero-dispersion propagation at s hort wavelengths,” Electron. Lett. 36, 514–515 (2000). 2. J. Riishede, J. Lægsgaard, J. Broeng, and A. Bjarklev, “Al l-silica photonic bandgap fibre with zero dispersion and a large mode area at 730 nm,” J. Opt. A 6, 667–670 (2004). 3. F. Luan, A. K. George, T. D. Hedley, G. J. Pearce, D. M. Bird, J. C. Knight, and P. St. J. Russell, “All-solid photonic bandgap fiber,” Opt. Lett. 29, 2369–2371 (2004). 4. A. Argyros, T. A. Birks, S. G. Leon-Saval, C. M. Cordeiro, F . Luan, and P. St. J. Russell, “Photonic bandgap with an index step of one percent,” Opt. Ex press 13, 309–314 (2005). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-13109. 5. P. Yeh, A. Yariv, and E. Marom, “Theory of Bragg fiber,” J. Opt . Soc. Am.68, 1196–1199 (1978). 6. J. C. Knight, J. Broeng, T. A. Birks, and P. St. J. Russell, “ Photonic Band Gap Guidance in Optical Fibers,” Science282, 1476–1478 (1998). 7. T. A. Birks, P. J. Roberts, P. St. J. Russell, D. M. Atkin, an d T. J. Shepherd, “Full 2-D photonic bandgaps in silica/air structures,” Electron. Lett. 31, 1941–1943 (1995). 8. J. Lægsgaard, “Gap formation and guided modes in photonic ba dgap fibres with high-index rods,” J. Opt. A 6, 798–804 (2004). 9. T. P. White, R. C. McPhedran, C. Martjin de Sterke, N. M. Litc hinitser, and B. J. Eggleton, “Resonance and scattering in microstructured optical fibers,” Opt. Lett. 27, 1977–1979 (2002). #101787 $15.00 USD Received 19 Sep 2008; revised 27 Oct 2008; accepted 27 Oct 2008; published 29 Oct 2008 (C) 2008 OSA 10 November 2008 / Vol. 16, No. 23 / OPTICS EXPRESS 18752 10. N. M. Litchinitser, A. K. Abeeluck, C. Headley, and B. J. E ggleton, “Antiresonant reflecting photonic crystal optical waveguides,” Opt. Lett. 27, 1592–1594 (2002). 11. A. Wang, A. K. George, and J. C. Knight, “Three-level neod ymium fiber laser incorporating photonic bandgap fiber,” Opt. Lett.31, 1388–1390 (2006). 12. V. Pureur, L. Bigot, G. Bouwmans, Y. Quiquempois, M. Douay, and Y. Jaouen, “Ytterbium-doped solid core photonic bandgap fiber for laser operation around 980 nm,” App l. Phys. Lett.92, 061113 (2008). 13. A. Isom̈aki and O. G. Okhotnikov, “Femtosecond soliton mode-locked la ser based on ytterbium-doped photonic bandgap fiber,” Opt. Express 14, 9238–9243 (2006). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-1420-9238. 14. G. Bouwmans, L. Bigot, Y. Quiquempois, F. Lopez, L. Provino , and M. Douay, “Fabrication and characterization of an all-solid 2D photonic bandgap fiber with a low-loss regi on (< 20 dB/km) around 1550 nm,” Opt. Express 13, 8452–8459 (2005). URLhttp://www.opticsexpress.org/abstract.cfm?URI=oe-132 -8452. 15. S. F́evrier, R. Jamier, J.-M. Blondy, S. L. Semjonov, M. E. Likhache v, M. M.Bubnov, E. M. Dianov, V. F. Khopin, M. Y. Salganskii, and A. N. Guryanov, “Low-loss singlemode la rge mode area all-silica photonic bandgap fiber,” Opt. Express14, 562–569 (2006). URLhttp://www.opticsexpress.org/abstract.cfm?URI=oe-142-562. 16. Y. Barannikov, A. Oussov, F. Shcherbina, R. Yagodkin, V. Gapontsev, and N. Platonov, “250 W, single-mode, CW, linearly-polarized fibre source in Yb wavelength range,” in Proceedings of Conference on Lasers and ElectroOptics (Optical Society of America, 2004), paper CMS3 (2004). 17. J. K. Lyngsø, B. J. Mangan, and P. J. Roberts, “Polarizati on maintaining hybrid TIR / bandgap all-solid photonic crystal fiber,” inProceedings of Conference on Lasers and Electro-Optics, and Conference on Quantum Electronics and Laser Science (Optical Society of America, 2008), paper CThV1 (2008). 18. R. Goto, K. Takenaga, K. Okada, M. Kashiwagi, T. Kitabaya shi, S. Tanigawa, K. Shima, S. Matsuo, and K. Himeno, “Cladding-Pumped Yb-Doped Solid Photonic Bandgap Fibe r for ASE Suppression in Shorter Wavelength Region,” inProceedings of Conference on Optical Fiber communication/National Fiber Optic Engineers Conference (Optical Society of America, 2008), paper OTuJ5 (2008). 19. A. Cerqueira. S. Jr., F. Luan, C. M. B. Cordeiro, A. K. Geor ge, and J. C. Knight, “Hybrid photonic crystal fiber,” Opt. Express14, 926–931 (2006). URLhttp://www.opticsexpress.org/abstract.cfm?URI=oe-142-926. 20. S. Johnson and J. Joannopoulos, “Block-iterative frequ ency-domain methods for Maxwell’s equations in a planewave basis,” Opt. Express 8, 173–190 (2001). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-8-3 -17 . 21. A. Argyros, T. A. Birks, S. G. Leon-Saval, C. M. B. Cordeir o, and P. S. J.Russell, “Guidance properties of low-contrast photonic bandgap fibres,” O pt. Express13, 2503–2511 (2005). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-137-2503. 22. T. A. Birks, F. Luan, G. J. Pearce, A. Wang, J. C. Knight, an d D. M. Bird, “Bend loss in all-solid bandgap fibres,” Opt. Express14, 5688–5698 (2006). URLhttp://www.opticsexpress.org/abstract.cfm?URI=oe-1412-5688. 23. L. Xiao, W. Jin, and M. S. Demokan, “Photonic crystal fibers confining light by both indexguiding and bandgap-guiding: hybrid PCFs,” Opt. Express 15, 15,637–15,647 (2007). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-1524-15637. 24. T. Hosaka, K. Okamoto, Y. Sasaki, and T. Edahiro, “Single mo de fibres with asymmetrical refractive index pits on both sides of core,” Electron. Lett. 17, 191–193 (1981). 25. N. A. Issa and L. Poladian, “Vector wave expansion method f or leaky modes of microstructured optical fibers,” J. Lightwave Technol. 21, 1005–1012 (2003). (Note that, in our paper, due to superior performance in most applications, a finite difference scheme is used in the radial direction instead of the basis function expansion described in the reference.) 26. X. Chen, M.-J. Li, N. Venkataraman, M. T. Gallagher, W. A. W ood, A. M. Crowley, J. P. Carberry, L. A. Zenteno, and K. W. Koch, “Highly birefringent hollow-core photonic b andgap fiber,” Opt. Express 12, 3888–3893 (2004). URL http://www.opticsexpress.org/abstract.cfm?URI=oe-1216-3888. 27. W. J. Bock and W. Urbanczyk, “Measurement of polarization mode dispersion and modal birefringence in highly birefringent fibers by means of electronically scanned shear ing-type inteferometry,” Appl. Opt. 32, 5841–5848 (1993). 28. M. S. Alam, K. Saitoh, and M. Koshiba, “High group birefrin gence in air-core photonic bandgap fibers,” Opt. Lett. 30, 824–826 (2005). 29. J. Noda, K. Okamoto, and Y. Sasaki, “Polarization-maintai ning fibers and their applications,” J. Lightwave Technol. 4, 1071–1089 (1983). 30. H.-T. Shang, “Chromatic dispersion measurement by white-l ight interferometry on metre-length single-mode optical fibres,” Electron. Lett. 17, 603–605 (1981).


Introduction
All-solid photonic bandgap (PBG) fibers [1][2][3][4] are one configuration of PBG fibers [5,6] in which a low-index glass core is surrounded by a microstructured cladding, which typically comprises isolated high-index glass regions embedded in a low-index glass background.The core-modes are guided not by total internal reflection (TIR) but by coherent multiple scattering from the microstructured cladding, and the guidance mechanism is explained by the PBG effect [7,8] or, more generally, by anti-resonant reflection [9,10].A particularly interesting aspect of all-solid PBG fibers is that their core can be doped with rare-earth ions to make fiber lasers.Such fiber lasers then benefit from the properties of all-solid PBG fibers, such as spectral filtering [11,12], chromatic dispersion adjustable by design [1,2,13], and the potential to achieve large mode area [2,14,15].
Many applications of all-solid PBG fibers in fiber lasers require birefringence and the capacity for efficient cladding pumping.For example, when a high power fiber laser is used for frequency doubling, linearly polarized output from a fiber laser is required, so that the laser cavity preferably consists of cladding-pumped birefringent fibers and a polarizer [16].To obtain high cladding pumping efficiency in all-solid PBG fibers, it is necessary to minimize the amount of pump power which is trapped (by index guiding) in the high-index regions, and hence not absorbed by the rare-earth doped core.It has been reported that birefringence in an all-solid PBG fiber can be realized by incorporating stress elements in a 2-D structure [17], however the reported structure has many high-index regions and therefore may suffer low cladding pumping efficiency.
With the aim of improving the cladding pumping efficiency of all-solid PBG fibers, we have previously reported a cladding-pumped, ytterbium-doped, all-solid hybrid microstructured fiber [18].The fiber is based on a recently reported new form of microstructured fiber, in which the guidance mechanism is based on both the PBG effect and TIR [19].The number of highindex regions is reduced more than ten times (from 126 to 12) compared to comparable 2-D structures, therefore high cladding pumping efficiency is expected.As a result of the twofold rotational symmetry of the fiber, birefringence is also expected.
In this paper, we report the characterization of an all-solid hybrid microstructured fiber having the same structure as previously reported [18] but having no ytterbium doping in the core.We measured modal birefringence of 1.5 × 10 −4 and group birefringence of 2.1 × 10 −4 at 1.31 µm, which are due to the twofold symmetry.The contribution of stress and form birefringence to the modal birefringence is discussed.The measured group birefringence showed large wavelength dependency near the edges of the second bandgap.We calculated the band structure of the 1-D arrangement of high-index regions and found it to differ noticeably from conventional 2-D PBG fibers.The bend loss was measured to show a strong directional dependence due to the coexistence of the two guiding mechanisms.The fiber has two important properties of PBG fibers; spectral filtering, and chromatic dispersion specific to PBG fibers.This structure is suitable for linearly-polarized, cladding-pumped fiber lasers utilizing the properties of PBG fibers.

Fiber structure
The cross section of the fiber is schematically shown in Fig. 1(a).In the silica cladding (shown in light gray), the Ge-doped high-index regions (shown in white) with pure silica jackets (shown in light gray) are positioned periodically in the x-direction with pitch Λ.The diameters of the high-index regions and pure silica jackets are d high and d si .The remainder of the cross section comprises fluoride(F)-doped low-index uniform glass (shown in dark gray).The core is formed by replacing one high-index region with pure silica and the core diameter is d core .Figure 1(b) shows the refractive index profiles along with the x-and y-axis of the fiber cross section.In the x-direction, the core is surrounded by the high-index regions and the guidance mechanism is based on the PBG effect.Along the y-axis, the core is surrounded by the low-index cladding and the guidance mechanism is based on TIR.The outer pure silica cladding surrounding the The cross section of the fabricated hybrid microstructured fiber is shown in Fig. 2. The stack and draw method was used for fiber fabrication.First, a Ge-doped silica preform with pure silica cladding and a uniformly F-doped silica preform were both drawn into rods.These rods were then hexagonally stacked in a pure silica tube and drawn to a fiber.The pitch of the high-index regions, Λ, is 8.0 µm.According to the measurement of the Ge-doped silica preform before being drawn into rods, ∆n high is about 2.8% and d high /Λ is ∼0.5.The relative refractive index profile of the high-index regions is approximated by ∆n(r) = ∆n high [1 − (r/R) 4.25 ], where r is the distance from the center of the high-index region and R = d high /2.The relative refractive index difference of the low-index cladding ∆n low is -0.35%.The fiber diameter is 148 µm.

Transmission
First, we measured the transmission spectrum of the fiber with different bend radii.The measurements were taken using a supercontinuum (SC) source and an optical spectrum analyzer (OSA).The fiber length was two meters and the input and output ends were fusion spliced to a step index fiber (λ cuto f f ∼ 0.95 µm) to measure core-modes.The fiber was coiled to three different radii; 160, 50, and 25 mm.For these measurements, no attention was paid to the bend direction of the fiber relative to the direction of the high-index regions.The transmission spectra of the fiber for the three different radii are shown in Fig. regard to the spectrum of the SC source.The second, third, and fourth bandgaps were observed in the wavelength regions centered at 1400, 900, and 700 nm.Additional but weaker transmission windows were observed between these bandgaps.These weak transmission windows are not observed in 2-D PBG fibers.They are sensitive to fiber bending, and almost disappear as the coiling radius is reduced.To analyze the origin of these weak transmission windows observed in Fig. 3, we calculated the band structures of the hybrid microstructured fiber and a conventional 2-D PBG fiber having the same high-index region.The plane wave expansion method [20] was used for the calculation.Material dispersion was neglected and the refractive index of pure silica was fixed to 1.45 for simplicity.To resemble the real structure, we assumed that d core and d si were both 8.8 µm in our calculations and hence we assumed the core and circular microstructural elements are overlapping by 0.8 µm.Λ, d high , ∆n(r), and ∆n low are the same as in the previous section.In Fig. 4(a), n e f f ∼ 1.445 corresponds to the refractive index of the F-doped low-index cladding and no bandgap exists below this line.Shown as a solid line is the fundamental core-mode in the second bandgap.The calculated transmission range is in reasonable agreement with the experiments, the difference may be attributed to the changes in the refractive index profile and shape when the preform was drawn to the fiber.When compared with the 2-D PBG structure [see Fig.  4(a)] between the second and third bandgaps.Indeed, poorly confined core-modes were found within the additional bandgap in our calculation and this explains the weak transmission window observed around 1100 nm in Fig. 3.The formation of this additional bandgap is explained by considering how bands are formed by high-index regions.Bands formed from high-index regions are determined by (1) the modes of each high-index region and (2) how high-index region modes couple and form a set of supermodes [8].According to this model, the set of supermodes between the second and third bandgaps is formed by the LP21 and LP02 modes of each high-index region.In the hybrid structure, high-index regions only exist in the x-direction, limiting the formation of broadband supermodes, and an additional bandgap appears between the LP21 and LP02 modes of the high-index regions.Figures 5(a It should be noted that the LP11 core-mode was found in the additional bandgap in our calculation, therefore the fiber may be multi-moded in the shorter wavelength region of the second bandgap.The results presented hereafter all relate to the fundamental mode because, in the experiments, a launch fiber was spliced to the hybrid fiber to excite only the core-modes of the fiber and the launch fiber is single-mode within the wavelength range of the measurements; the fundamental core-mode of the hybrid fiber was therefore selectively excited.Figure 7 shows the loss spectrum of the fiber in the second bandgap.A minimum loss of 8 dB/km was measured at 1300 nm using a 66 m-length fiber, which was spooled on a 160 mmdiameter bobbin.We believe that the measured loss is sufficiently low for most fiber laser applications.The loss increase around 1240 and 1380 nm originates from OH ions, as no special care was taken to reduce OH content in the fiber during fiber fabrication.

Bend loss
The fiber should have two bend loss mechanisms, relating to each of the guidance mechanisms.To confirm this, we measured the directional dependency of bend loss of this fiber.The experimental setup is shown in Fig. 8.A half-turn bend was applied to a 1 m-length fiber using a mandrel (Radius = 12.5 mm) and the bend loss was measured as a function of the bend angle θ .The results are shown in Fig. 9.When θ = 0 • , almost no bend loss was observed, because the dominant mechanism of bend loss is that of fibers guided by TIR and TIR is still maintained.On the other hand, when θ = 90 • , significant bend loss appeared at both short and long wavelength edges of the transmission range, because the dominant mechanism of bend loss is now that of all-solid PBG fibers and the bend changed the band structure of the fiber [21].This property may practically be beneficial to reduce bend loss of all-solid PBG fibers, if the fiber (or its coating) has a non-circular shape which forces the fiber to be bent in the θ = 0 • direction.We next qualitatively compare the bend loss of the hybrid fiber with a comparable 2-D PBG fiber by comparing the band structures.By comparing Fig. 4 structure has deeper bandgaps, i.e., has large bandgaps in the direction of the effective index.The deeper bandgaps are realized by reduced mode coupling between the high-index regions and give the fiber reduced bend loss [22].To understand the bend loss sensitivity, we consider two cases, θ = 0 • and 90 • .When θ = 0 • , the origin of the bend loss is similar to fibers guided by TIR, thus the refractive index difference between the core-modes to the low-index cladding [shown in Fig. 4(a) as ∆n e f f ] is a good measure of bend loss sensitivity.When θ = 90 • , the origin of the bend loss is similar to PBG fibers, thus the refractive index differences between the core-modes to the nearest supermodes (shown in Fig. 4 as ∆n + e f f and ∆n − e f f ) is a good measure of bend loss sensitivity [22].In both cases, these differences are larger for the hybrid microstructured fiber compared to the 2-D PBG fiber.This suggests that this hybrid fiber should show reduced bend sensitivity compared to the 2-D PBG fiber regardless of the bend angle θ .

Birefringence
The hybrid microstructured fiber has only twofold symmetry, so that the fiber has both form birefringence [23] and stress birefringence [17].The stress birefringence of the hybrid microstructured fiber arises from the one-dimensionally arranged highly Ge-doped regions, which have a higher thermal expansion coefficient compared to pure silica.
Modal birefringence is generally the most important parameter for a polarization maintaining fiber (PMF) since it is a direct measure of the ability to maintain linear polarization.When both stress and form birefringence contribute to the birefringence, the total modal birefringence (B m ) is the sum of the modal birefringence due to stress birefringence (B ms ) and form birefringence (B m f ), i.e., The B m of the fiber was measured by a cut-back method [24].Linearly polarized light (polarized at 45 • relative to the x-axis of the fiber) was launched into the core of the fiber.A single-mode launch fiber was spliced to the input end of the fiber to excite the fundamental core-mode.We used a short launch fiber (less than 5cm) and kept it straight so that the change of the polarization state in the launch fiber is minimized.A rotatable polarizer was positioned at the output of the fiber, and the degree of linear polarization (DOLP) at the output was determined by finding the angles where the maximum and minimum output are obtained.DOLP is defined by where I max and I min in Eq. ( 2) are the maximum and minimum output power through the polarizer.The fiber length was initially 1 m and was shortened by 500 µm or 1 mm in each polarization measurement, and the DOLP was measured as a function of the removed fiber length.For this measurement, we used a laser diode operating at 1.31 µm, which is nearly at the center of the second bandgap.Figure 10 shows the measured DOLP as a function of the removed fiber length.A DOLP oscillation with a period of ∼4.5 mm is observed, which indicates the beatlength is 9 mm.The beatlength corresponds to modal birefringence of 1.5×10 −4 at 1.31 µm.The measured modal birefringence is comparable to that of conventional PMFs so this fiber can be used as a PMF.To analyze the origin of the modal birefringence, we also calculated the B m f using the ABC-FDM method [25].The calculated B m f , however, was of the order of 10 −6 in the middle of the bandgap and the difference between this value and the measurement is more than an order of magnitude.We believe that the measured mode birefringence is primarily related to the B ms arising from the high-index regions at this wavelength.
We measured the group birefringence by the fixed analyzer method and the Jones matrix eigenanalysis (JME).For the fixed analyser method, broadband light from a SC source was launched into the fiber through a polarizer and the output from the fiber was detected by an OSA after another polarizer.We used a 2 m-length fiber.Two single-mode fibers with negligible birefringence were spliced to both ends of the hybrid microstructured fiber to selectively measure the fundamental core-mode.Figure 11(a) shows the measured spectrum.The measured spectrum was not normalized and the dip around 1400 nm is due to the output spectrum of the SC source.Figure 11(a) shows the measured power as a function of the wavelength; the oscillation is due to the birefringence of the fiber.This oscillation is clearly shown in the detailed spectra in Figs.11(b) and (c).The group birefringence B g (λ ) is given by where L is the length of the fiber, λ is the wavelength, and ∆λ is the wavelength difference between two peaks of the oscillation [26].Interestingly, the period of the oscillation becomes very large around 1160 nm and 1540 nm.This implies that the group birefringence becomes zero and changes sign around these two wavelengths.Taking this into account, we calculated the group birefringence using Eq. ( 3).The result is shown in Fig. 11(d) as a blue curve.The group birefringence changes sign quite smoothly at these two wavelengths, supporting the assumption that the group birefringence becomes zero.The two red curves shown in Fig. 11(d  The difference between the measured modal and group birefringence in the middle of the bandgap is relatively large.In addition, the measured group birefringence changes sign near the edges of the bandgap.These results are quite different from conventional PMFs such as PANDA or Bow-Tie fibers, in which the difference between the two birefringence values is very small [27], and the group birefringence has the same sign within the entire operating wavelength range.To analyze these two unusual results, consider the definition of group birefringence (B g ) which is given by, Equation (4) shows that B m and B g can differ significantly when dB m /dλ is large, i.e., when B m is highly wavelength dependent.The measured difference between B m and B g is therefore attributed to the relatively large wavelength dependence of B m in the middle of the bandgap.The large wavelength dependency of B m could be both due to stress and form birefringence.By substituting Eq. (1) into Eq.( 4), we obtain where #101787 -$15.00USD Received 19 Sep 2008; revised 27 Oct 2008; accepted 27 Oct 2008; published 29 Oct 2008 (C) 2008 OSA

#
101787 -$15.00USD Received 19 Sep 2008; revised 27 Oct 2008; accepted 27 Oct 2008; published 29 Oct 2008 (C) 2008 OSA low-index cladding is far from the core and the leakage loss through the low-index cladding is negligibly small.

Fig. 1 .
Fig. 1.Schematic cross section and refractive index profile of all-solid hybrid microstructured fiber.

Fig. 4 .
Fig. 4. Calculated band structure and fundamental core-mode of the hybrid and 2-D structure.The core-mode is shown only in the second bandgap for simplicity.7×7 supercell is used for the calculation.

Figures 4 (
Figures 4(a) and (b) show the band structures of the hybrid and 2-D PBG fibers.In Fig.4(a), n e f f ∼ 1.445 corresponds to the refractive index of the F-doped low-index cladding and no bandgap exists below this line.Shown as a solid line is the fundamental core-mode in the second bandgap.The calculated transmission range is in reasonable agreement with the experiments, the difference may be attributed to the changes in the refractive index profile and shape when the preform was drawn to the fiber.When compared with the 2-D PBG structure [see Fig.4(b)],it is seen that the hybrid structure has an additional bandgap [region surrounded by the dotted Figures 4(a) and (b) show the band structures of the hybrid and 2-D PBG fibers.In Fig.4(a), n e f f ∼ 1.445 corresponds to the refractive index of the F-doped low-index cladding and no bandgap exists below this line.Shown as a solid line is the fundamental core-mode in the second bandgap.The calculated transmission range is in reasonable agreement with the experiments, the difference may be attributed to the changes in the refractive index profile and shape when the preform was drawn to the fiber.When compared with the 2-D PBG structure [see Fig.4(b)],it is seen that the hybrid structure has an additional bandgap [region surrounded by the dotted ) and (b) show two typical intensity profiles of the supermodes between the second and additional bandgaps; Figs.6(a) and (b) show the intensity profiles of the supermodes between the third and additional bandgaps.In the figures, the border of the pure silica jackets and the low-index F-doped cladding is shown as solid lines.As the figures clearly show, the band of supermodes between the second and additional bandgaps is formed by the LP02-based supermodes, and that between the third and additional bandgaps is formed by the LP21-based supermodes.These additional bandgaps may be eliminated by a modified design.In our calculations, as we increased d high /Λ, the high-index regions became more coupled and the additional bandgap disappeared.

Fig. 5 .Fig. 6 .
Fig. 5. Typical intensity profiles of the LP02-based supermodes between the second and additional bandgaps of the hybrid structure.

Fig. 10 .
Fig. 10.Measured DOLP as a function of removed fiber length.
) are the measured group birefringence by the JME using a 2 m-length fiber.The wavelength #101787 -$15.00USDReceived19Sep 2008; revised 27 Oct 2008; accepted 27 Oct 2008; published 29 Oct 2008 (C) 2008 OSArange was limited by the availability of tunable light sources.The sign of the measured group birefringence was changed accordingly, based on our assumption that the group birefringence becomes zero and changes sign around 1540 nm.These two results are in good agreement.It should be noted that the sign of the group birefringence is not determined by these experimental methods, thus the sign is arbitrary in Fig.11(d).